MATERIALS SCIENCE Chameleon-like elastomerswith · PDF file MATERIALS SCIENCE Chameleon-like...
Embed Size (px)
Transcript of MATERIALS SCIENCE Chameleon-like elastomerswith · PDF file MATERIALS SCIENCE Chameleon-like...
Chameleon-like elastomers with molecularly encoded strain-adaptive stiffening and coloration Mohammad Vatankhah-Varnosfaderani,1 Andrew N. Keith,1* Yidan Cong,1* Heyi Liang,2* Martin Rosenthal,3 Michael Sztucki,3 Charles Clair,4 Sergei Magonov,5
Dimitri A. Ivanov,6,7 Andrey V. Dobrynin,2† Sergei S. Sheiko1†
Active camouflage is widely recognized as a soft-tissue feature, and yet the ability to integrate adaptive coloration and tissuelike mechanical properties into synthetic materials remains elusive. We provide a solution to this problem by uniting these functions in moldable elastomers through the self-assembly of linear-bottlebrush-linear triblock copolymers. Microphase separation of the architecturally distinct blocks results in physically cross-linked networks that display vibrant color, extreme softness, and intense strain stiffening on par with that of skin tissue. Each of these functional properties is regulated by the structure of one macromolecule, without the need for chemical cross-linking or additives. These materials remain stable under conditions characteristic of internal bodily environments and under ambient conditions, neither swelling in bodily fluids nor drying when exposed to air.
T he mechanical and optical properties of bi- ological tissues emerge fromdistinct physi- cal origins but act in concert to serve living organisms such as chameleons, cephalopods, and amphibians (1–3). For example, initial-
ly soft and compliant tissues such as skin stiffen rapidly during deformation to prevent injury. Within narrow intervals of strain, their elastic
moduli increase by several orders of magnitude at rates far beyond those observed for conven- tional elastomers, gels, and thermoplastics (Fig. 1, A to C). These tissues may also simultaneously convertwhite light into colorful patterns through constructive interference with light waves co- herently scattered by periodic or quasi-periodic structures (Fig. 1D) (4). Collectively, these func-
tions constitute defense and signaling mecha- nisms that have inspired the design of various biomimetic materials that either have tissue- likemechanics (5–11) or display structural colors (12–14). However, integrating both attributes into themolecular structure of a singlematerial proves to be extremely challenging. Themechanics of biological tissues arise from
their composite nature, defined by the distinct mechanical response of two proteins, collagen and elastin (15). A scaffold of stiff collagen fibers resists deformation, and an interwoven elastin network ensures elastic recoil. This structural duet produces a characteristic, two-phase me- chanical response (16), beginningwith exponen- tial stiffening and switching to a linear response (strue ~ l, where strue is the true stress and l is the elongation ratio) halfway before the point of rupture, as exhibited by plotting differentialmod- ulus @strue/@l as a function of l (Fig. 1B). The
Vatankhah-Varnosfaderani et al., Science 359, 1509–1513 (2018) 30 March 2018 1 of 5
Fig. 1. Distinct mechanics and colora- tion of biological tissue. (A) A schematic of materials’ true stress–elongation curves demonstrates the diversity of possible mechanical responses and the intense strain stiffening of initially soft tissue. Apparent Young’s modulus E0 is determined as the tangent of a stress- strain curve at l = 1. L, length of the sample at a given instant; L0, initial length of the sample. (B and C) Differential modulus of biological tissues and synthetic materials (tables S6 and S7). bb, bottlebrush; Synt., synthetic; PU/AM, polyurethane/acrylamide hydrogel. (D) Color variation in the skin of a male panther chameleon changing from a relaxed to an excited state. [Adapted from (1)] (Insets) Transmission electron micros- copy images of the guanine nanocrystal lattice from the same individual in the corresponding states.
1Department of Chemistry, University of North Carolina at Chapel Hill, Chapel Hill, NC 27599, USA. 2Department of Polymer Science, University of Akron, Akron, OH, 44325-3909, USA. 3European Synchrotron Radiation Facility, F-38043 Grenoble, France. 4Université de Haute Alsace, Laboratoire de Physique et Mécanique Textiles, F-68093 Mulhouse Cedex, France. 5Scanning Probe Microscopy (SPM) Labs, Tempe, AZ 85283, USA. 6Institut de Sciences des Matériaux de Mulhouse-IS2M, CNRS UMR 7361, F-68057 Mulhouse, France. 7Lomonosov Moscow State University, Faculty of Fundamental Physical and Chemical Engineering, Leninskie Gory 1/51, 119991 Moscow, Russian Federation. *These authors contributed equally to this work. †Corresponding author. Email: [email protected] (A.V.D.); s[email protected] (S.S.S.)
on A ugust 19, 2021
ow nloaded from
resulting sigmoid shape of the @strue/@l curves contrasts with the steady increase in stiffness displayed by synthetic elastomers and gels (Fig. 1C). Although variousmolecular andmacroscopic constructs implement the basic principles of strain stiffening (6–11), none replicate tissue’s deforma- tion response completely and precisely. For ex- ample, various silicone rubbers, such as Ecoflex and Dragon Skin, which are widely used in or- thotics and cinematography (17), have skinlike softness but lack the strain-stiffening character- istics of skin (Fig. 1C). Polymeric gels are simi- larly incapable of replicating tissue mechanics (Fig. 1C) and further suffer from solvent leakage upon deformation (18). We simultaneously enhanced softness and
strain stiffening in recent work by employing brushlike architecture in solvent-free elastomers (Fig. 1C) (19). The attachment of side chains to network strands yielded a dual mechanical ef- fect: Moduli were reduced to 100 Pa via chain disentanglement, and strain stiffening increased by an order of magnitude via strand extension due to side-chain steric repulsion (20). Although this effect enablesmechanical replicas of gel-like tissues such as lung and jellyfish (5), the strain stiffening of these systemspaleswhen compared with that of soft connective tissues like skin. In parallel, various chromogenic polymers have been created (21–23), but they fail to incorporate
tissuelike mechanical properties. This conven- tional divide presents amaterial design challenge aimed at mimicking skin tissue—soft on touch, stiff upon deformation, and colored for appeal or camouflage. We report the design of chromogenic elasto-
mers, formed bymicrophase separation of linear- bottlebrush-linear ABA triblock copolymers (Fig. 2A), that are solvent free, supersoft (apparent Young’smodulusE0 ~ 10
3 to 105 Pa), and strongly strain stiffening ðE�10 @[email protected] ∼ 1 to 102Þ. We ex- plored the symbiosis of two blocks that are both chemically and physically distinct: (i) flexible linear chains that aggregate into rigid domains and (ii) stiff bottlebrush strands that form a supersoft matrix. This interplay of the attributes of rigid-while-flexible and soft-while-stiff, which are oxymoronic upon first glance, is actually rep- resentative of the distinctive potential of archi- tectural control over materials’mechanical and optical properties. Elucidating howboth building blocks not only play individual roles in this con- trol but also synergizewith each other to enhance biomimetic performance is a central feature of this study. Specifically, we show that aggregation of linear blocks yields physical networks, and bottlebrush strands provide these networks with a lowmodulus. Further, the strong segregation of the chemically dissimilar blocks (24) augments the architectural prestrain of the bottlebrush blocks
(20) and therebymarkedly improves the networks’ strain-stiffening characteristics (fig. S15). These effects enable replication of the mechanical re- sponse of porcine skin and achieve substantial progress toward replicating that of human skin, as discussed below. To validate this concept, we have synthesized
several series of linear-bottlebrush-linear ABA triblock copolymers with different degrees of po- lymerization (DPs; represented asn) of the bottle- brush backbone (nbb≈ 300 to 1800) and identical DPs of the polydimethylsiloxane (PDMS) side chains (nsc = 14) (Fig. 2A, fig. S1 to S3, and table S1). Each series containsmoleculeswith different DPs of the linear Ablock (nA≈80 to 1200) correspond- ing to A-block volume fractions ðfAÞ of 0.03 to 0.3, where the A blockmay be poly(methylmeth- acrylate) (PMMA), poly(benzyl methacrylate) (PBzMA), or poly(oligo(ethylene glycol) mono- methyl ether methacrylate) [P(OEOMA)]. For physical tests, thin filmswere prepared by solution casting. During solvent evaporation, microphase separation results in thermoplastic elastomers (plastomers) with characteristic coloration pro- duced by constructive interference with light waves reflected by domain interfaces (Fig. 2B andmovie S1). Both color and mechanical prop- erties depend on plastomer morphology, which was characterized by differential scanning calo- rimetry (DSC) and atomic forcemicroscopy (AFM)
Vatankhah-Varnosfaderani et al., Science 359, 1509–1513 (2018) 30 March 2018 2 of 5
Fig. 2. Structural coloration of plastomers. (A) Self-assembly of linear-bottlebrush-linear ABA triblock copolymers yields physical networks—A domains of linear blocks embedded in a B matrix of bottlebrush strands, where nA, nbb, and nsc are degrees of polymerization (DPs) of the linear block, the bottlebrush backbone, and the bottlebrush side chains, respectively. The microphase-separated structure is described in terms of the interbrush distance (d1), the diame- ter of the spherically shaped PMMA domains (d2), and the interdomain distance (d3)